### UNIVERSIT ` A DEGLI STUDI DI PARMA DIPARTIMENTO DI FISICA

### Spin dynamics in magnetic molecules

### Studio delle dinamiche di spin in sistemi molecolari magnetici

### Alberto Bianchi

*Thesis submitted for the award of the degree of Ph.D. in Physics*
Dottorato di Ricerca in Fisica

### Supervisor: Prof

^{.}

### Paolo Santini

XXI ciclo - Gennaio 2009

This document was typeset in Adobe^{r} Utopia and Computer Modern Roman
by the author using the L^{A}TEX2ε software.

The file in Portable Document Format was generated with pdfTEX version 13c.

Copyright 2009 by Alberto Bianchi. All Rights Reserved.c

Author’s address Alberto Bianchi

Dipartimento di Fisica

Universit`a degli Studi di Parma

Viale G. P. Usberti 7/A, I-43100 Parma, Italy E-mail: mailto:alberto.bianchi@fis.unipr.it

to my mother and my brother, my endless present to my father and my grandparents, my sweet memories to Irida, my sunny future

iii

iv

## Contents

1 Introduction 3

1.1 Magnetic Molecules . . . 5

1.2 The archetipal nanomagnet: Mn_{12} . . . 6

1.3 Beyond the Mn_{12} nanomagnet . . . 10

2 Theoretical description of molecular magnets 13 2.1 The spin Hamiltonian. . . 13

2.2 Spin Hamiltonian: Main Contributions . . . 16

2.3 Spin Hamiltonian: a perturbative approach . . . 20

2.4 Strong exchange limit. . . 21

3 Spin dynamics in magnetic molecules: experimental techniques 25 3.1 Inelastic Neutron Scattering . . . 25

3.2 Nuclear Magnetic Resonance . . . 30

3.2.1 Perturbative treatment of the hyperfine dipolar interaction between nuclear and electronic spins . . . 35

4 Neutron spectroscopy and magnetization study of Cr_{8}Zn and Cr_{8}Cd 37
4.1 Rotational band picture in rings and spin segments . . . 38

4.2 Theory . . . 39

4.3 Inelastic neutron scattering experiments . . . 43

4.4 Discussion . . . 46

4.5 Magnetization study of Cr_{8}Cd . . . 49

4.6 Conclusions . . . 55

5 Macroscopic measurements in Cr_{7}Ni and Cr_{8}Ni 57
5.1 The Cr_{7}Ni heterometallic ring. . . 58

5.2 The Cr_{8}Ni heterometallic ring . . . 59

5.3 Conclusions . . . 70

6 Relaxation dynamics in magnetic molecules 73 6.1 Decoherence and relaxation phenomena in magnetic molecules . . . 73

6.2 The Mn12 and Fe8 nanomagnets . . . 78

6.3 The Fe_{30} mesoscopic molecule . . . 85

6.3.1 Nuclear magnetic resonance measurements . . . 86

6.3.2 Theoretical analysis and discussion . . . 87 v

6.4 The antiferromagnetic cluster V_{12}.. . . 93
6.5 The antiferromagnetic ring Cr_{7}Ni. . . 95
6.6 Conclusions . . . 100

7 General conclusions 103

A Inelastic and quasi-elastic components of spin dynamics 107

vi

## List of Figures

1 Structure of the Mn_{12} cluster. . . 6

2 Level diagram within the ground multiplet S = 10 of Mn_{12}. . . 7

3 Relaxation time τ of magnetization in the Mn_{12} cluster. . . 9

4 Hysteresis loop measured on a Mn_{12} monocrystal at T =2.1 K. . . 10

5 The full Hamiltonian matrix representing all the magnetic interactions. 20 6 Typical time scales of spin dynamics in molecular magnets. . . 26

7 Representation of the experimental set up for a time of flight (tof ) direct geometry spectrometer. . . 28

8 The structure of a Cr_{8}Zn molecule. The hydrogen atoms have been
omitted for clarity. . . 38

9 Effects of breaking or ring symmetry in Cr8Zn spin segment. . . 40

10 Energy of the low-lying triplet eigenstates for Cr8 and Cr8Zn. . . 42

11 Cr_{8}Zn INS spectra collected with λ=7 and 3.8 ˚A. . . 45

12 INS spectra as a function of the scattering vector amplitude Q.. . . 48

13 Schematic views of Cr_{8} (closed ring) and Cr_{8}Cd (open ring). . . 49

14 Magnetization curves of Cr_{8}Cd and Cr_{8} molecules. . . 51

15 Magnetization curves at T =1.3 K for Cr_{8}. . . 52

16 ∆H_{n} as a function of n. . . 53

17 Local magnetic moments for Cr_{8} and Cr_{8}Cd. . . 55

18 View of the structure of a Cr_{7}Ni molecule. . . 58

19 Magnetization curve of Cr7Ni and derivative dM/dH. . . 59

20 Schematic view of Cr8Ni compound.. . . 60

21 Temperature dependence of magnetic susceptibility in Cr_{8}Ni. . . 61

22 Magnetization measurements and calculations in Cr_{8}Ni. . . 62

23 H-dependence of ∆H for Cr_{8}Ni compound.. . . 63

24 H-dependence of the specific heat at T =0.5 K for Cr_{8}Ni. . . 64

25 Temperature dependence of full width of half amplitude (FWHA) of
1H-NMR spectra in Cr_{8}Ni. . . 65

26 Effect of sizeable DM interactions in energy levels of a Cr_{8}Ni molecule. 68
27 Quantum and classic correlation functions in the Cr8Ni compound. . . 69

28 One of the degenerate configurations corresponding to an S = 0 ground
state for the classical version of the model of Cr_{8}Ni. . . 70

29 Structure of spin eigenstates in a Cr_{8}Ni molecule. . . 71
vii

30 Calculated frequency weights A(λ, T, B) of the magnetization autocor-

relation function vs 1/T in Mn_{12}. . . 78

31 Relaxation time in the Mn_{12} cluster vs H_{z}. . . 80

32 Measured and calculated out-of-phase susceptibility and magnetization
relaxation time in the Fe_{8} nanomagnet. . . 81

33 Breakdown of the Arrhenius law in the Fe_{8} nanomagnet. . . 82

34 Dominant relaxation time in the Fe_{8} molecule as a function of H_{z} and
1/T . . . 83

35 Effects of the fast intra-well relaxation mechanism in the Fe_{8} nanomagnet. 84
36 1/T_{1}/(χT ) vs T curves for Fe_{30} cluster. . . 87

37 The two lowest bands of energy levels calculated for Fe_{30}. . . 88

38 Relaxation properties of a Fe_{30} magnetic molecule.. . . 91

39 Schematic representation of the V_{12} cluster. . . 93

40 Spin dynamics in the V_{12} molecule. . . 95

41 Reduced proton NMR 1/T_{1}/(χT ) for Cr_{7}Ni molecule. . . 96

42 Calculated and measured proton NMR 1/T_{1}/(χT ) and spectrum of mag-
netization fluctuations for the Cr_{8} compound. . . 98

43 Measured and calculated reduced proton 1/T_{1}/(χT ) as a function of T
for the Cr_{8} compound. . . 99

44 T -dependence of the calculated 1/T_{1}/(χT ) for the Cr_{7}Ni cluster. . . 100
45 A characteristic Lorentzian centered in ω_{kn} and of FWHM given by 2γ_{nk}.110

viii

Summary

In questo lavoro sono stati sviluppati modelli teorici nell’ambito dell’approccio spin Hamiltoniana al fine di studiare le dinamiche di spin coerente e incoerente in varie classi di molecole magnetiche. Questi sistemi sono formati da un core di ioni magneti- ci, tipicamente ioni di metalli di transizione, circondato da ligandi organici. I ligandi organici impediscono un’interazione effettiva tra i cores, mentre all’interno di un core i diversi spin sono fortemente accoppiati tra loro da interazioni di superscambio. In particolare, nella classe dei cosiddetti nanomagneti molecolari l’interazione tra gli ioni

`

e cos`ı forte, che a bassa temperatura ciascuna molecola si comporta come una parti-
cella magnetica a spin totale fissato in presenza di un potenziale effettivo. In questi
sistemi, la dinamica coerente, caratterizzata da scale di tempo brevi, `e coinvolta in
vari fenomeni quantistici di interesse fondamentale (come il tunneling della magnetiz-
zazione). La dinamica incoerente, che implica scale di tempo pi`u lunghe, ricopre un
ruolo fondamentale dal momento che rappresenta l’ostacolo principale per le potenziali
applicazioni tecnologiche delle molecole magnetiche come memorie ad alta densit`a o
come bit quantistici. Nel presente lavoro, la dinamica coerente `e stata studiata diret-
tamente mediante l’analisi e l’interpretazione di misure di scattering anelastico di neu-
troni, e, indirettamente, attraverso l’analisi di misure di bulk (come magnetizzazione
e calore specifico ad alti campi). In questo modo `e stato inoltre possibile studiare
le interazioni microscopiche alla base delle dinamiche di spin descritte all’interno di
Hamiltoniane di spin microscopiche. I relativi parametri sono stati determinati dal
confronto tra teoria ed esperimenti quali scattering anelastico di neutroni, suscettivit`a
magnetica, calore specifico e magnetizzazione. In particolare, sono stati determinati i
parametri microscopici (dello scambio, dei campi cristallini, dell’interazione dipolare)
dell’Hamiltoniana microscopica della molecola denominata Cr_{8}Zn. Trattandosi di un
anello aperto il Cr_{8}Zn rappresenta un sistema modello per lo studio delle conseguenze
della rottura della simmetria ad anello. Conseguenze di tale rottura si trovano non
solo nel diagramma dei livelli energetici, ma anche nella struttura degli autostati e si
riflettono in particolare nelle misure di scattering anelastico di neutroni in funzione
del momento trasferito. Inoltre, mediante l’analisi di misure macroscopiche sono state
determinate le Hamiltoniane microscopiche di anelli antiferromagnetici come il Cr_{7}Ni,
il Cr_{8}Cd e il Cr_{8}Ni. Quest’ultimo in particolare, essendo un sistema magneticamente

2 _{Summary}

frustrato, ha permesso di investigare a fondo le conseguenze della frustrazione magnet-
ica nella dinamica quantistica. Per quanto riguarda la dinamica di rilassamento, vari
tipi di molecole magnetiche sono stati presi in considerazione: i ben noti nanomagneti
Mn_{12} e Fe_{8}, la molecola icosidodecaedrica Fe_{30}, il sistema antiferromagnetico V_{12} e il
noto anello antiferromagnetico Cr_{7}Ni. Nel caso dei nanomagneti si `e mostrato come
raffreddando il campione e applicando un campo magnetico sufficientemente grande si
pu`o velocizzare la dinamica di rilassamento della magnetizzazione, facendo cos`ı venire
meno la nota legge di Arrhenius. Per il Fe_{30}, il V_{12} e il Cr_{7}Ni l’analisi della dinamica
di rilassamento `e supportata da misure NMR. Si `e provato come nei primi due casi
le misure NMR restituiscono direttamente informazioni sulla dinamica di rilassamento
della magnetizzazione. Per l’anello eterometallico Cr_{7}Ni, invece, misure di NMR di
1/T1 restituiscono informazioni sulla dinamica di osservabili molecolari non diretta-
mente riconducibili alla magnetizzazione. In tutti e tre i casi l’analisi delle dinamiche
di spin conduce a un ottimo accordo tra le misure NMR e le relative predizioni teoriche.

Il modello sviluppato per lo studio delle dinamiche di spin, dunque, coglie gli aspetti fondamentali alla base dei fenomeni di rilassamento.

## Chapter 1 Introduction

Molecular Magnetism is an interdisciplinary area in Condensed Matter Research which brings together Chemists and Physicists to the major challenge of investigating the magnetic properties of matter. Magnetic molecules have been intensively studied so far because of their potential technological applications and for the possibility they offer to investigate fundamental properties of matter at the nanoscopic scale. These systems contain a core of magnetic ions (typically 3d transition metal ions) surrounded by organic ligands. Molecules are embedded in a crystal structure with the organic lig- ands preventing interaction among the cores. On the other hand, the magnetic ions within a core are usually strongly coupled through superexchange interactions. Since the interaction between clusters is negligible, effects related to a single molecule can be probed by means of bulk techniques. An intensively studied class of magnetic molecules is constituted by the so called single molecule magnets (shortly, SMMs) or molecular nanomagnets [1,2,3]. These systems are characterized by a slow relaxation of magne- tization at low T and give rise to magnetic hysteresis. This is one condition for storing information in a molecule. Therefore, since a SMM represents an isolated magnetic entity, it might be considered as the smallest practical unit for magnetic memories.

This would increadibly increase the amount of information storable with respect to current devices. There are other classes of molecules (antiferromagnetic rings, grids, mesoscopic molecules . . . ) for which the envisaged technological applications cover the fields of quantum computation and magnetorefrigeration. In order to have a deeper un- derstanding of fundamental features and a major control on technological aspects, the spin dynamics constitutes the key point. Both from a theoretical and an experimental point of view, the spin dynamics is characterized by two distinct regimes: coherent and incoherent. At short times it is the coherent spin dynamics which gives rise to

3

4 1. Introduction

quantum effects in magnetic molecules, such as the quantum tunneling of magnetiza-
tion. Furthermore, the ability to control this dynamics turns out to be crucial to carry
out logic gates for quantum computing. On the other hand, the incoherent part of
spin dynamics involves longer times, tipically of the order of 10^{−6} s ore more at low
temperature. The understanding of relaxation mechanisms is fundamental since relax-
ation and more generally decoherence constitute a major obstacle to the technological
applications of magnetic molecules in the fields of high density memory storage and
quantum computation.

This thesis is organized as follows. In the next sections, a brief introduction on molecu- lar nanomagnets will be given, with particular attention to the relaxation mechanisms which characterize the dynamics of magnetization in the prototype of these systems, the so called Mn12 [1]. Chapter 2 will focus on the spin Hamiltonian approach here followed to theoretically describe magnetic molecules. The typical microscopic inter- actions in magnetic molecules will be taken into account, and a general expression of the molecular spin Hamiltonian will be given in terms of tensor operators [4,5,6,2].

Chapter 3 will be devoted to the experimental techniques most of the theoretical re-
sults refer to, i.e. inelastic neutron scattering (INS) and nuclear magnetic resonance
(NMR). Chapters 4, 5, 6 will summarize the main results of this thesis on the static
and dynamic magnetic properties of these materials [7,8,9,10,11]. The coherent part
of spin dynamics has been directly investigated through analysis of inelastic neutron
scattering (INS) data, and indirectly through analysis of macroscopic measurements
such as magnetization and specific heat. In Chapter 4, the microscopic spin hamilto-
nian of Cr_{8}Zn compound has been determined by comparing the experimental cross
sections with theoretical predictions. The nature of elementary excitations in open spin
segments has been thus clarified and is apparent in experimental data. Macroscopic
magnetization measurements at high fields carried out for the parent Cr_{8}Cd compound
corroborate the results obtained from neutron spectroscopy. This proves that the spin
hamiltonian approach gives a good description of incoherent spin dynamics even for
spin multiplets not accessible to the INS technique. The same holds for the case of
Cr_{7}Ni, a cluster which has been shown to be a good candidate for quantum computing.

In Chapter5magnetization measurements on Cr_{7}Ni confirm the picture derived in ex-
isting interpretation of INS data. Besides, in this chapter macroscopic measurements
on another heterometallic ring named Cr_{8}Ni have been analyzed. This compound is
magnetically frustrated and has offered the unique opportunity of investigating the
effects of frustration on quantum dynamics. As regards relaxation phenomena, several

1.1. Magnetic Molecules 5

molecules have been taken into account in Chapter6: the Mn_{12} and Fe_{8} nanomagnets,
the Fe_{30} icosidodecaedron, the V_{12} antiferromagnetic cluster containing ions with spin
1/2 and the already mentioned Cr_{7}Ni heterometallic ring. The incoherent dynamics on
nanomagnets has been intensively studied in recent years, but non completely under-
stood. Fe_{30}represents a mesoscopic molecule of great fundamental interest. V_{12} shows
an anomalous behaviour in NMR data. At last, the study of the relaxation dynamics in
Cr_{7}Ni is crucial for the envisaged application of the molecule as a qubit. In all studied
clusters, there is a good agreement between available data and calculations and thus
the theory captures the main features of relaxation phenomena.

Finally, in Chapter7general conclusions will be given with particular consideration on future perspectives and developments of the here presented research activity.

### 1.1 Magnetic Molecules

A magnetic molecule is a system containing a finite number of magnetic centers (transi- tion metal ions, rare-earth ions, organic radicals) which are ferro- or antiferro- magneti- cally coupled through superexchange pathways [2,6]. Shells of organic ligands sorround each cluster preventing effective inter-cluster interactions. Thus, each molecule can be considered as an isolated magnetic entity. A nanomagnet can be defined as a system that shows slow relaxation of the magnetization of purely molecular origin. Under the so called blocking temperature [2,12] a magnetic cluster behaves as a nanomagnet giv- ing rise to magnetic hysteresis of purely molecular origin. This is the reason for which these systems have also been named single molecule magnets. A SMM has dimensions small enough to show fascinating quantum effects such as the quantum tunneling of magnetization (or QTM). This phenomenon is the magnetic analogue of the tunneling of an α particle in a radioactive nucleus. The magnetic moment is aligned along the easy-axis, and changes its orientation by tunneling through the energy barrier. In re- cent years there has been an enormous progress in chemical techniques to synthetize new compounds with all envisaged properties: number of interacting spins, type of metallic centers, amount and kind of anisotropy, and so on.

Beyond information storage, magnetic molecules have been thought as building blocks
for quantum computing. For instance, a system with an S = 1/2 ground state can
be regarded as a qubit, or quantum bit, the quantum analogue of the classic bit, and
used to implement algorithms of quantum computation. One of the best candidates
for this purpose has been proved to be the heterometallic ring known as Cr_{7}Ni [13],

6 1. Introduction

**High-frequency EPR spectra of a molecular nanomagnet:**

**Understanding quantum tunneling of the magnetization**

Anne Laure Barra

*Laboratoire des Champs Magnetiques Intenses, CNRS, Boite Postale 166, Grenoble Cedex 9, France*

Dante Gatteschi and Roberta Sessoli

*Department of Chemistry, University of Florence, Via Maragliano 75, 0144 Firenze, Italy*

~Received 31 January 1997!

EPR spectra have been recorded in very high fields up to 25 T, and at high frequency up to 525 GHz, on a
polycrystalline sample of @Mn12O_{12}~CH3COO!16~H2O!4#•2CH3COOH•4H2O ~Mn12ac!, a molecular cluster
behaving like a nanomagnet. The simulation of the spectra has provided an accurate determination of the
*parameters of the spin Hamiltonian H*5m*B***H****•g•S1D@S***z*

2*21/3S(S11)#1B*_{4}^{0}*O*_{4}^{0}*1B*_{4}^{4}*O*_{4}^{4}*, where O*_{4}^{0}*535S*_{z}^{4}
*230S(S11)S**z*2*125S**z*2*26S(S11)13S*^{2}*(S*11)^{2} and *O*_{4}^{4}*51/2(S*_{1}^{4}*1S*_{2}^{4}*): D*520.46(2)cm^{21},
*B*_{4}^{0}522.2(2)310^{25} cm^{21}*, and B*_{4}^{4}564(1)310^{25} cm^{21}. The presence of the fourth-order term in the total
spin justifies the irregularities in the spacing of the jumps, recently observed in the hysteresis loop of Mn12ac
and attributed to acceleration of the relaxation of the magnetization due to quantum tunneling between degen-
*erate M states of the ground S510 multiplet of the cluster. The term in (S*_{1}^{4}*1S*_{2}^{4}) is responsible for the
transverse magnetic anisotropy and plays a crucial role in the mechanism of quantum tunneling. The high-
frequency-EPR spectra have shown its presence and quantified it.@S0163-1829~97!08237-4#

**I. INTRODUCTION**

Quantum tunneling of the magnetization~QTM! is one of
the candidates to test the possibility of observing quantum
effects in macroscopic ~or perhaps more appropriately meso-
scopic! objects.^{1,2} The interest for this kind of problem is
certainly a theoretical one, aimed at understanding the limits
of validity of quantum mechanics, but in principle also a
practical one. In fact small magnetic particles are used to
store information and it would be desirable to have a knowl-
edge of the lower limit of the size which can be achieved.

The requisite for storing information is that the magnetiza-
tion is either up or down, but if tunneling occurs, the stored
information is lost. Therefore the limit size for observing
QTM should be known.^{3}

Many attempts were made to produce even smaller
magnets,^{4,5} but most efforts were plagued by the impossibil-
ity of obtaining ensembles of identical nanoparticles which
could be kept well separated from each other in order to
minimize interactions which would hamper the observation
of QTM. Techniques of molecular chemistry on the other
hand suggested a different approach, using large molecular
clusters as single nanomagnets.^{6} Surprisingly enough it was
found that nanomagnetic properties can be observed in rela-
tively small clusters, comprising only eight metal ions.^{7}

The main advantage that molecular clusters have com-
pared to other systems, like small magnetic particles either of
metals or of oxides, or even ferritin, is that they are abso-
lutely monodisperse, their structure is perfectly known from
x-ray techniques, they can be well separated one from the
other by dissolving them in appropriate solvents and polymer
films.^{8,9}

The most accurately investigated system so far is

@Mn12O_{12}~CH3COO!16~H2O!4#•2CH3COOH•4H2O, Mn12ac,
which has the structure shown in Fig. 1. It comprises an

external ring of eight manganese*~III! ions (S52) and an*
internal tetrahedron of four manganese*~IV! ions (S53/2).*

*The cluster has a crystal imposed S*_{4} symmetry.^{10} It has a
*ground S*510 state, which can be loosely described setting
all the manganese*~III! spins up (S5832516) and all the*
manganese*~IV! spins down (S52433/2526). The*
ground multiplet is split by the tetragonal symmetry to leave
*the M*5610 components lying lowest.^{11}At low temperature
these are the only populated levels.

Mn12ac is a molecular cluster for which slow relaxation
of the magnetization was detected at low temperature,^{11}
similar to the blocking temperature of superparamagnets. In
fact, the relaxation time was found to follow a thermally
activated behavior down to 2 K, according to the equation
t5t0*exp(A/kT), with a pre-exponential factor* t052.1
310^{27} *s, and an energy barrier A/k*561 K.^{12} In this range
of temperature the cluster behaves like a single-molecule

FIG. 1. Sketch of the structure of the magnetic core of the clus-
*ter. The arrows show the spin structure of the ground S*510 state.

PHYSICAL REVIEW B VOLUME 56, NUMBER 13 1 OCTOBER 1997-I

56

0163-1829/97/56~13!/8192~7!/$10.00 8192 © 1997 The American Physical Society

Figure 1: Structure of the Mn12cluster. The outer ring is formed by eight ions Mn(III) with four unpaired electrons and spin 2, whilst the inner four ions Mn(IV) have three unpaired electrons and thus spin 3/2. Arrows indicate the configuration of the ground state of the molecule, a multiplet S = 10.

which shows an effective S = 1/2 ground state well separated by excited levels. It
has also been demonstrated how magnetic molecules can be used as magnetocaloric
refrigerants at low temperature. It is the case of another Chromium-based magnetic
ring named Cr_{7}Cd [14]. Both Cr_{7}Ni and Cr_{7}Cd were derived by the well known Cr_{8}
compound, a fact which demonstrates the possibility of tuning the properties of mag-
netic molecules by a chemical substitution of magnetic centers. We will see in the next
chapters how this possibility will turn out to be extremely useful in order to evaluate
the consequences of the various types of breaking of ring symmetry.

### 1.2 The archetipal nanomagnet: Mn

_{12}

In the early nineties, it was discovered that the dodecanuclear compound [Mn12O12(CH

3COO)_{16}(H_{2}O)_{4}], shortly Mn_{12}[15], shows a slow relaxation behaviour of magnetization
at low temperature. It has been theoretically and experimentally demonstrated that
the time characterizing the thermally activated relaxation process in the interval 2-15
K follows an Arrhenius law:

τ = τ_{0}exp( ∆

k_{B}T) (1)

1.2. The archetipal nanomagnet: Mn12 7

left and right well, giving rise to a so-called tunnel splitting, D_{T}
(Figure 1 b). One of the two coupled levels is of lower energy
than the degenerate levels, while the other is of higher energy,
exactly like a pair of bonding±antibonding levels in elemen-
tary MO theory. The possibility of tunneling is related to the
relative energies of the tunnel splitting and of the barrier. The
smaller the ratio between the two the smaller the possibility of
observing tunneling.

So far we have considered the system of the particle in the
two wells as completely separated from the environment. This
is clearly an approximation, because the interaction with the
environment can be minimized, but not
completely eliminated. If the particle is
localized in a metastable state (Fig-
ure 2), it can tunnel out of the metasta-
ble state. No energy is involved if the
particle is isolated from the environ-
ment, whereas coupling to the environ-
ment means that the particle loses
energy with the tunneling (as shown by
the arrows in Figure 2). The interactions
with the environment will tend to local-
ize the particles, because the interactions will make one well
more ™attractive∫ than the other (that is, reduce the energy of
one of the wells). In the case of strong coupling with the
environment, which means that this interaction is much larger
than the tunnel splitting, the particle will stay localized in one
of the two wells, and will not tunnel. For intermediate
coupling the particle can tunnel, but jumping incoherently
from one well to the other. This means that one particle will
tunnel, and localize for some time in the other well, and then
tunnel again, but in an irregular way. The third case is that of
weak coupling when the tunnel splitting is large compared to
the interaction with the environment, and the particle
oscillates coherently between the two minima. The conditions
for observing coherent tunneling are severe. Evidence for
coherent tunneling is the observation of energy absorption at
a frequency corresponding to the tunnel splitting. In the
above experiment of calyx[4]arene a peak was observed in the
proton-spin lattice-relaxation rate at a field corresponding to
the tunneling frequency of 35 MHz.^{[25]}

In the above discussion we did not take into account the
origin of the interaction between the two wavefunctions. It is
apparent that in the description we have made some implicit
assumptions: 1) that an unperturbed Hamiltonian, h0, gives
the initial description with the two equivalent wells, 2) a
perturbation Hamiltonian, h_{1}, is added which couples the
two separate states and removes the degeneration, 3) a
Hamiltonian describing the interaction with the environment,
h_{2}, is needed [Eq. (1)].

h¼ h0þ h1þ h2 ð1Þ

The actual form of the three relevant Hamiltonians will depend on the nature of the system taken into consideration.

In this article we will be focussing on magnetic systems, therefore we will limit the description to such systems.

3. Magnetic Relaxation in Systems with Large Spin

Let us consider a system with a well defined ground spin
state, characterized by a large value of S (for example Mn12ac
with S¼ 10). The unperturbed Hamiltonian includes the
effect of an external magnetic field parallel to the unique axis
of the cluster and of its axial splitting as a result of crystal-field
effects. At this level of approximation only the second-order
crystal-field effects will be included. Therefore, for the
discussion we wish to develop,^{[26]} the h0 Hamiltonian can
be written as Equation (2) where D is a negative constant for
the system of interest and H_{z}is the magnetic field strength in
the z direction. D is one of the parameters of the so-called
Zero Field Splitting (ZFS) because it removes the degeneracy
of the S multiplet.

h_{0}¼ D ½S^{2}_{z}SðS þ 1Þ=3 þ g BHzSz ð2Þ

The energies of the spin levels corresponding to h_{0}are in
fact easy to calculate as given by Equation (3), whereS
MS S.

EðM_{S}Þ ¼ D ðM^{2}_{S}110=3Þ þ g _{B}MSHz ð3Þ

The energy levels can be plotted as shown in Figure 3 a.

When no external field is applied all the levels are degenerate
pairs, except MS¼ 0. Since D is negative the MS¼ S levels
will lie lowest. In Figure 3 the states with positive MS are
plotted in one potential well, and those with negative M_{S}in
the other. This formalism is an extension of that commonly
used for superparamagnets (see below).^{[27]}A system like this
is characterized by magnetic anisotropy along the ™easy axis∫,
which means that the magnetization is preferentially oriented
parallel to the z axis.

Figure 2. Tunneling from a metastable state.

Figure 3. Energy levels for a spin state S with easy axis magnetic aniso- tropy. The þM levels are localized in the left well and the M levels in the right well. a) In zero field the two wells are equally populated;

b) the application of a magnetic field selectively populates the right well; c) after removing the field the return to equilibrium occurs through a series of steps.

Single-Molecule Magnets

**Angewandte**

**Angewandte**

**Chemie**

271

Angew. Chem. Int. Ed. 2003, 42, 268 ± 297

Figure 2: Level diagram within the ground multiplet S = 10 of Mn12 as inferred from Eq. (2). Levels with M > 0 and with M < 0 are localized in the left and in the right potential hole respectively. (a): At zero magnetic field the two groups of levels are equally populated. (b): The application of a magnetic field selectively populates the right hand hole. (c): After the removal of the magnetic field the system returns back to equilibrium through multi-step Orbach processes.

with τ_{0}=2.1×10^{−7} and _{k}^{∆}

B=61 K [16,17,18]. It can be argued that at 2 K it takes
several months for the magnetization to relax back to equilibrium. This behaviour
results from thermally activated multi-step Orbach processes as shown in Fig. 2. At
low temperature, i.e. T < 2 K, measurements of the relaxation time τ shows that the
Arrhenius law is not satisfied and τ tends to a finite value when T → 0. This has
been interpreted as a QTM involving the two lowest levels. This phenomenology can
be well understood by analyzing the interactions which govern the low T behaviour
of the spin dynamics of the Mn_{12} molecule. In order to give a complete theoretical
description of Mn12 one should explore the complete Hilbert spin space spanned by
the twelve spins: the eight outer Mn(III) ions with spin s_{a}=2, and the four inner
Mn(IV) ions with spin s_{b}=3/2. The computation of the number of spin levels would
give (2s_{a}+ 1)^{8}× (2sb+ 1)^{4} = 10^{8}. As a result, an exact spin Hamiltonian approach is
unfeasible even though modern computing machines are exploited. For many purposes,
it is sufficient to describe the spin dynamics of the molecule at low T , by observing that
the antiferromagnetic (AFM) exchange interactions among the eight Mn(III) and the
four Mn(IV) ions lead to a S = 10 ground multiplet. Fig. 1represents the arragement
of the twelve ions in the ground state of the molecule: the Mn(III) ions have their spins
pointing in the upward direction, while the other Mn(IV) ions point downward [1,19].

8 1. Introduction

At low T the Mn_{12} cluster can be well described within the ground S = 10 multiplet
by an unperturbed Hamiltonian which includes the effects of the crystal field up to
second order:

H_{0} = D[S_{z}^{2}− S(S + 1)/3] + gµBH_{z}S_{z}, (2)

where the second term represents the coupling with a magnetic field H_{z}, taken along
the z direction, which is the easy axis of magnetic anisotropy, g≈ 2 and µBis the Bohr
magneton. The level diagram can be easily obtained from the above hamiltonian, and
the levels

E(M_{S}) = D(M_{S}^{2}− 110/3) + gµBH_{z}M_{S} (3)

with H_{z} = 0 are shown in Fig. 2(a). In absence of an applied magnetic field, levels with
M_{S} =±S constitute the degenerate ground doublet. Besides, levels with MS > 0 and
M_{S} < are supposed to be in the left and in the right side of the double well potential
respectively. Though the above hamiltonian contains only the axial part of 2nd order
crystalline anisotropy, some aspects of the thermally activated relaxation mechanisms
in the temperature range 2-15 K can be well understood. Let us suppose to prepare the
system in a magnetized state [see Fig. 2(b)] by the application of a magnetic field along
the z-axis. If T is low and H_{z} applied on the z-axis strong enough, only the M_{S} =−10
state is populated. Thus the cluster magnetization reaches the saturation value. At the
removal of the field, the molecule will be out of thermodynamic equilibrium: in fact, at
zero field the two ground M_{S} =±S states are degenerate and as a consequence should
be equally populated. The system returns back to equilibrium thanks to the coupling
of the spins with other degrees of freedom. At T > 1 K the most important source
which causes relaxation processes is constituted by phonons [20,21]. The spin phonon
interaction has its main origin in a perturbation of the crystal fields induced by lattice
vibrations. The effects of such a perturbation are experienced by each magnetic ion and
can be taken into account in terms of a spin-phonon hamiltonian, whose leading terms
are second order spin operators. Therefore, transitions between|MS > and|MS± 1 >,

|MS ± 2 > are allowed. For the sake of simplicity, at this level only transitions with
selection rule|∆M| = |MS− MS^{0}| = 1 will be considered. As a consequence, a spin flip
may occure from, say, MS =−10 to MS =−9, if the molecule absorbs a quantum of
energy corresponding to the energy difference E(M_{S} =−9) − E(MS =−10). In order
to relax back to equilibrium, i.e. a spin-flip between |MS >= −10 and |MS >= 10,
consecutive transitions from adiacent levels have to be performed [see Fig. 2(c)]. This is

1.2. The archetipal nanomagnet: Mn12 9

Figure 3: Relaxation time τ of magnetization in the Mn12cluster as a function of mag- netic field applied along the easy axis. At given fields τ shows sharp minima and the system undergoes a faster relaxation mechanism: the quantum tunneling of magnetiza- tion. Measurements were made at T = 5 K [17].

the phonon-induced mechanism which takes place through multi-step Orbach processes.

Another relaxation mechanism has been found in Mn_{12} which is a clear manifestation
of the quantum mechanical nature of this spin system and, in general, of SMMs: the so
called quantum tunneling of magnetization (QTM). Fig. 3shows the relaxation time τ
as a function of magnetic field applied along z, the easy axis of magnetization. It can
be observed that τ increaseas up to H = 1.5 KOe, where it reaches a maximum, then
it decreases again showing minima at H = 4.5 KOe and H = 8.5 KOe. This behaviour
was completely unexpected: in fact, in traditional superparamagnets the relaxation
time diminishes in a monotonic way when H increases since the magnetic anisotropy
barrier progressively reduces. The QTM novel phenomenon can be understood if in
the Hamiltonian (2) further crystal field terms allowed by the tetragonal symmetry of
the cluster ^{1} are taken into account:

H_{S=10}= D

3O_{2}^{0}+ B_{4}^{0}O_{4}^{0}+ B_{4}^{4}O_{4}^{4}. (4)

The above hamiltonian contains CF contributions up to fourth order. In particular, the last term represents a weak transverse anisotropy and removes the degeneracy between

1The here reported microscopic parameters were determined by means of inelastic neutron scat-
tering experiments: D=-0.457 cm^{−1}, B_{4}^{0}=-2.33×10^{−5} cm^{−1}, B^{4}_{4}=±3 × 10^{−5} cm^{−1} [22].

10 1. Introduction

Figure 4: Hysteresis loop measured on a Mn12monocrystal at T =2.1 K. At anticrossing fields the hysteresis shows sharp steps due to the QTM between the couples of quasi- degenerate levels. In correspondence of each anticrossing the relaxation of magnetization becomes faster and a steps occurs.

levels M_{S} =±10, MS =±6 and MS =±2 thus allowing the tunneling of magnetization
to manifest. The occurrence of clear minima in τ at particular magnetic fields in Fig.

3 can be explained if the Zeeman term H_{Zeeman} = gµ_{B}H_{z} is added in Eq. (4). At
given magnetic fields, a couple of levels becomes quasi-degenerate and a so called
anti-crossing takes place. In correspondence with these anticrossing fields the system
is subjected to a faster relaxation since the involved levels allow a thermally assisted
quantum tunneling. This explaines the behaviour shown in Fig. 3. Consequences of the
thermal assisted QTM phenomenon are directly seen in magnetization measurements.

In Fig. 4 an hysteresis loop measured at T =2.1 K on a Mn_{12} monocrystal is shown.

In correspondence of an anticrossing field a thermally assisted QTM occurs between the quasi degenerate pair of levels. The magnetization has not to overcome the overall double-well potential to relax back to equilibrium, indeed tunnels it and the relaxation process becomes faster. This is the origin of the steps in the hysteresis loop, which it is worth to rembember is an effect of purely molecular origin.

### 1.3 Beyond the Mn

_{12}

### nanomagnet

There are several reasons behind the great efforts researchers devote to the synthesis of new types of magnetic molecules and to the investigation of their magnetic properties.

Some of these reasons are the potential technological applications envisaged in the fields
of information storage, quantum computation and magnetorefrigeration [2,16,23]. In
order to have molecules which are suitable to be used as high-density memories, a high
blocking temperature T_{B}is needed [2,12], at least higher than the helium melting point.

1.3. Beyond the Mn12 nanomagnet 11

In fact, the height of the barrier potential stabilizes the sample magnetization against
thermal disorder. Therefore, a large U is required to have a high T_{B}: for this purpose
a molecule with a high spin ground state is needed together with a large Ising-type
anisotropy. The magnetic molecule with the highest energy barrier observed so far is
the Mn_{6} cluster, with U ≈ 86.4 K. Nonetheless, it is insufficient for technological ap-
plications. In fact, since the τ0 in the prefactor of Eq. (1) is very small, magnetization
blocking only occurs below about 4.5 K [24]. Since in conventional SMMs the energy
barrier seems difficult to be significantly increased, other compounds have been taken
into account. In particular, the new family of lanthanide single molecule magnets has
gained great attention [25,26,27,28,29].

As regards the field of quantum computation, one of the best candidates to be used as a qubit has been proved to be the Cr7Ni compound [13]. This is a Chromium-based heterometallic ring, in which magnetic centers are antiferromagnetically coupled [30].

This molecule was obtained from the well-know homometallic ring Cr_{8} by substitution
of a Cr^{3+} ion (s=3/2) with a Ni^{2+} ion (s=1). While in Cr_{8} the compensation of anti-
ferromagnetic interactions leads to a singlet S = 0 ground state, in Cr_{7}Ni the ground
Kramers doublet S = 1/2 accounts for the presence of a Ni^{2+} ion. In Ref. [13] it has
been demonstrated that at low T Cr7Ni well behaves as an effective two level system.

In fact, the S-mixing between the ground state doublet |S = 1/2 > and higher levels

|S > 1/2 > (<1%) is low enough that transitions between |S = 1/2 > and |S > 1/2 >

induced by transverse field required in qubit manipulation are negligible.

The last of the above mentioned technological applications of magnetic molecules lies in the field of magnetorefrigeration [31]. Recent results demonstrate that the magne- tocaloric effect can be exploited in a Chromium based cluster named Cr7Cd at tem- peratures T < 2 K [14].

12 1. Introduction

## Chapter 2

## Theoretical description of molecular magnets

In order to give a theoretical description of magnetic clusters we exploit the irreducible tensor operator (ITO) technique.

### 2.1 The spin Hamiltonian

A magnetic molecule formed by a number N of magnetic ions can be described in terms of the following spin Hamiltonian:

H = H_{0}+ H_{CF} + H_{DIP}, (5)

where H_{0} is the isotropic Heisenbgerg-Dirac interaction, H_{CF} represents the local
crystal fields while H_{DIP} contains both the dipolar intracluster interaction and the
anisotropic exchange. In general, other terms may compare in Eq. (5), such as the
antisymmetric, biquadratic and anisotropic exchange as we will see in the next section.

Here Eq. (5) gathers the usually leading interactions in the spin Hamiltonian of a magnetic molecule. The three contributions of Eq. (5) can be written as:

H0 = X

i>j

Ji,jsi· sj (6)

H_{CF} = X

i

X

k,q

b^{q}_{k}(i)O_{k}^{q}(s_{i}) (7)

H_{DIP} = X

i>j

s_{i}· Dij · sj, (8)

where s_{i} is the spin operator of the ion on i-th site, J_{ij} are the isotropic exchange
integrals, and D_{ij} is the second order dipolar tensor, usually evaluated within the

13

14 2. Theoretical description of molecular magnets

point dipole approximation [32]. The second term represents the local crystal fields
(CFs), with O^{q}_{k}(s_{i}) Stevens operator equivalents for the i-th ion [6,33,34], and b^{q}_{k}(i)
CF parameters. Here k = 2, 4 for d electrons and k = 2, 4, 6 for f electrons [6], while
q =−k, . . . , k. The total dimensions of the Hamiltonian matrix is:

D =

N

Y

i=1

(2s_{i}+ 1). (9)

Depending on the values of N and s_{i} D can be very large. For instance, D = 2^{4} = 16
for V_{12}, but this value is enormous for Fe_{30} for which D = 6^{30}, of the order of the
Avogadro’s number. In order to represent the interactions of Eq. (5), it is natural the
choice of the product states

|s1m_{1}i |s2m_{2}i · · · |sNm_{N}i

as basis functions. Nonetheless, H_{0} is often the dominant term in Eq. (5). Thus
a better choice of the basis states is constituted by the eigenstates of the total spin
S = P

is_{i}. Besides, an appropriate coupling schemes is to be chosen. For a cluster
with N magnetic ions with spins S1, S2, . . . , SN a successive coupling scheme leads to
the following basis vectors:

s1s2( ˜S2)s3( ˜S3)...sN −1( ˜SN −1)sNSM E

=

( ˜S)SM E

(10)
where ( ˜S) represents the complete set of intermediate spin quantum numbers ˜S_{k}, with
k = 1, . . . , N− 1. Here the first intermediate spin ˜S2 = S12 is given by the coupling of
s_{1} with s_{2}. Then ˜S_{2} is coupled to s_{3} to have ˜S_{3} = S_{123} and so on. For a system with
N ions N − 1 is the number of required intermediate spins to specify each possible
spin state. Different choices can be made as regards the coupling scheme. Anyway,
all coupling schemes are equivalent, since the corresponding representative vectors are
connected to each other by a given unitary transformation. It is wise to remark that
it is much more convenient to choose a coupling scheme which reflects the symmetries
of the molecular system. The eigenstates|vi of H will be given by linear combinations
of the basis states

( ˜S)SME :

|vi = X

( ˜S)SM

D

( ˜S)SM vE

( ˜S)SME

, (11)

where the coefficients D

( ˜S)SM vE

can be evaluated once the spin-Hamiltonian of the system has been diagonalized. The irreducible tensor operator (ITO) technique allows

2.1. The spin Hamiltonian 15

to exploit the total spin symmetry of the cluster and to simplify both analytical and
numerical calculations [32,35]. Since each term of Eq. (5) can be rewritten as a
combination of tensor operators T^{(k)}, the generalized spin-Hamiltonian of a magnetic
molecule is:

H_{c} = X

k1,k2,...,kN

X

˜k2,...,˜kN

X

kq

C_{q}^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{2}), k_{N})×

× Tq^{(k)}(k1, k2, ˜k2, ..., kN −1, (˜kN −1), kN) (12)
where −k ≤ q ≤ k, Tq^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N}) is the q-th component of the
ITO of rank k, which can be decomposed in terms of ITO’s S_{q}^{k}^{i}

i(i)≡ Sq^{k}i^{i} defined in the
subspace of each single spin (k_{i}=0,1, . . . , 2s_{i}):

T_{q}^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N}) =

(

n

...S^{k}^{1} ⊗ S^{k}^{2} ^{˜}k2

⊗ S^{k}^{3}o^{˜}^{k}^{3}
...

)k^{˜}_{N −1}

⊗ S^{k}^{N}

k

q

. (13)

In the above expression the symbol ⊗ denotes the tensor product and ˜k2 = k_{12}, ˜k_{3} =
k_{123}, . . .. Besides, by expoliting the Wigner decomposition the values the intermediate
rank ˜k2 assumes are:

˜k_{2} = k_{1}+ k_{2}, k_{1}+ k_{2}− 1, . . . , |k1− k2| ,

and so on for the other intermediate ranks ˜k_{i}. At this point, if the Hamiltonian H_{c}of the
spin system is known, the eigenvalue problem has to be solved in order to calculate all
physical observables we are interested in. Therefore, the matrix elements of operators
Tq^{(k)} have to be calculated within the basis states. By exploiting the Wigner-Eckart
theorem [5] we have:

D

( ˜S^{0})S^{0}M^{0}

T_{q}^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N})

( ˜S)SME

=

= (−1)^{S}^{0}^{−M}^{0}D

( ˜S^{0})S^{0}

T^{k}

( ˜S)SE S^{0} k S

−M^{0} q M

(14)

where

S^{0} k S

−M^{0} q M

is a 3-j symbol and D

( ˜S^{0})S^{0}

T^{k}

( ˜S)SE

is the reduced matrix element between the two states. Finally, by means of successive decoupling procedures, this reduced matrix element can be expressed in terms of single spin reduced matrix elements and 9-j coefficients:

D
( ˜S^{0})S^{0}

T^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N})

( ˜S)SE

=

16 2. Theoretical description of molecular magnets

S_{N}

S^{k}^{N}
S_{N}

N −1

Y

1

q

(2k_{i+1}+ 1)(2 ˜S_{i+1}+ 1)(2 ˜S^{0}_{i+1}+ 1) +

S_{i}||Si^{k}||Si

k˜i ki+1 ˜ki+1

S˜^{0}_{i} S^{0}_{i+1} S˜^{0}_{i+1}
S˜_{i} S_{i+1} S˜_{i+1}

, (15)

where the ...

are the 9-j symbols. For k = 0, 1, 2 the single spin reduced matrix elements are:

S

S^{(0)}

S =p

(2S + 1)δS,S^{0} (16)

S

S^{(1)}

S =p

S(S + 1)(2S + 1)δ_{S,S}^{0} (17)

S

S^{(2)}

S = 1

√6

p(2S + 3)(2S + 1)(S + 1)S(2S− 1)δS,S^{0} (18)

### 2.2 Spin Hamiltonian: Main Contributions

After the generalized spin-Hamiltonian formalism has been introduced, it is necessary to focus on the main physical interactions which determine the spin-Hamiltonian and to rewrite them in terms of the ITO’s.

First of all, the exchange part of the spin-Hamiltonian is to be introduced:

H_{EX} = H_{0}+ H_{BQ}+ H_{AS} + H_{AN}. (19)

The first term H_{0} is the Heisenberg-Dirac Hamiltonian, which represents the isotropic
exchange interaction, H_{BQ} is the biquadratic exchange Hamiltonian, H_{AS} is the an-
tisymmetric exchange Hamiltonian, and, finally, HAN representes the anisotropic ex-
change interaction. Convetionally, they can be expressed as follows [1,6]:

H_{0} = X

i>j

J_{i,j}s_{i}· sj (20)

H_{BQ} = X

i>j

j_{i,j}(s_{i}· sj)^{2} (21)

H_{AS} = X

i>j

G_{i,j} · [si× sj] (22)

H_{AN} = X

i>j

X

α=x,y,z

J_{i,j}^{α}s^{α}_{i}s^{α}_{j}, (23)

where J_{i,j} e J_{i,j}^{α} are the parameters of the isotropic and anisotropic exchange interac-
tions respectively, j_{i,j} are the coefficients of the biquadratic exchange interaction, and,

2.2. Spin Hamiltonian: Main Contributions 17

finally, G_{i,j} =−Gj,i is the vector of the antisymmetric exchange. For the sake of sim-
plicity, further low symmetry terms in the anisotropic exchange and more complicated
terms between three or more spin centers in the biquadratic exchange interaction have
been neglected [35]. The magnetic dipole-dipole interaction can be taken into account
within the above exchange contributions [1]. In fact, both terms contain the same
dependence on spin operators and differ only as regards the coefficients J_{ij}^{α}.

The terms of the spin-Hamiltonian above can be written in terms of the ITO’s. By exploiting the properties of the angular momentum, the following relations can be found:

s^{x}(i) = S_{−1}^{(1)}(i)− S1^{(1)}(i)

√2

s^{y}(i) = iS_{−1}^{(1)}(i) + S_{1}^{(1)}(i)

√2

s^{z}(i) = S_{0}^{(1)}, (24)

where the Sq^{(1)}, q = 0, 1, 2, are the first rank irreducible tensors acting in the spin-spaces
of individual ions. By means of the above relations and of the Wigner decomposition
we have [35]:

H_{0} =−√
3X

i>j

J_{i,j}T_{0}^{(0)}(11|ij) (25)

where T_{0}^{(0)}(k_{i}k_{j}|i, j) describes the isotropic exchange interaction between a couple of
spins, and can be obtained from T^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N}) by substituting the
corresponding values of ki and kj, and by imposing kl=0 ∀ 6= i, j. Furthermore, the
following expressions can be obtained:

HBQ = −X

i>j

ji,j[√

5T^{(0)}(22|ij) +

√3

2 T^{(0)}(11|ij)] (26)

H_{AS} = −i√
2X

i>j

X

q

(−1)^{q}G^{(1)}_{q,ij}T_{−q}^{(1)}(11|ij) (27)

where

G^{(1)}_{q,ij} =

( _{∓(G}

x,ij√±iG_{y,ij})

2 if q =±1
G_{z,ij} if q = 0
and:

H_{AN} =X

i>j

J_{i,j}^{a} T^{(0)}(11|ij)+X

i,j

J_{i,j}^{u} [T_{2}^{(2)}(11|ij)+T−2^{(2)}(11|ij)]+X

i,j

J_{i,j}^{v} T_{0}^{(2)}(11|ij)(28)

18 2. Theoretical description of molecular magnets

where the parameters of anisotropic exchange are given by
J_{i,j}^{a} =− 1

√3(J_{i,j}^{x} + J_{i,j}^{y} + J_{i,j}^{z} )
J_{i,j}^{u} = 1

√2(J_{i,j}^{x} − J_{i,j}^{y} )
J_{i,j}^{v} = 1

√6(2J_{i,j}^{z} − Ji,j^{x} − Ji,j^{y} ),

and in the biquadratic term a costant term has been neglected.

As it can be seen in Eqs. (26), (28), both the biquadratic and the anisotropic Hamil-
tonians contain a scalar rank-0 contribution, i.e. T^{(0)}(11|ij). This two terms can be
incorporated in the isotropic exchange Hamiltonian by defining the effective isotropic
parameters as ˜J_{i,j} = J_{i,j}+ ^{1}_{3}(J_{i,j}^{x} + J_{i,j}^{y} + J_{i,j}^{z} ), thus having

H_{0} =−√
3X

i>j

J˜_{i,j}T_{0}^{(0)}(11|ij). (29)

As a result, the biquadratic and anisotropic Hamiltonians become:

H_{BQ} =−√
5X

i>j

j_{i,j}T^{(0)}(22|ij) (30)

HAN = 1

√2 X

i>j

J_{i,j}^{u} [T_{2}^{(2)}(11|ij) + T−2^{(2)}(11|ij)] +X

i,j

J_{i,j}^{v} T_{0}^{(2)}(11|ij). (31)

In order to complete the description of the spin system, contributions to the spin Hamiltonian due to local crystal fields (CFs) are to be taken into account [6,33,34].

By exploiting the same procedure, also the local CFs can be written in terms of the ITO’s. The Hamiltonian describing the interaction of the magnetic ions with their CFs can be written as:

H_{CF} =X

i

X

k,q

b^{q}_{k}(i)O^{q}_{k}(s_{i}) (32)

with O^{q}_{k}(s_{i}) Stevens operator equivalents for the i-th ions and b^{q}_{k}(i) CF parameters [6].

For transition metal ions k = 2 or 4 (larger values are forbidden for d electrons [6]),
and q =−k, . . . , k. The Stevens operator equivalents acting on site j can be expressed
in terms of ITO’s with all k_{i}’s equal to zero apart from k_{j}. As an example, the widely
used second order Hamiltonian

H_{CF} =X

i

d_{i}(s^{2}_{z}(i)− s_{i}(s_{i}+ 1)

3 ) +X

i

e_{i}(s^{2}_{x}(i)− s^{2}y(i), (33)

2.2. Spin Hamiltonian: Main Contributions 19

in terms of single site ITO’s can be rewritten as:

H_{CF} =X

i

d_{i}
r2

3T_{0}^{(2)}(i) +X

i

e_{i}(T_{2}^{(2)}(i) + T_{−2}^{(2)}(i)). (34)
The two terms of the above equation are the axial and rhombic part of crystal field
anisotropy. The Tq^{(k)}(i) operators describe the single ion crystalline anisotropy and can
be obtained from T^{(k)}(k1, k2, ˜k2, ..., kN −1, (˜kN −1), kN) by imposing ki=k and kl=0 ∀l6=i.

Besides, it is worth to remark that from Eq. (14) the expression for the matrix element of a generic rank-k tensor operator is:

D

( ˜S^{0})S^{0}M^{0}

T_{q}^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N})

( ˜S)SME ∝ S^{0} k S

−M^{0} q M

. Therefore, from the definition of 3-j symbols and exploiting the properties of the an- gular momenta addition rules through Clebsh-Gordan coefficients [5,36,37], we have:

D

( ˜S^{0})S^{0}M^{0}

Tq^{(k)}(k_{1}, k_{2}, ˜k_{2}, ..., k_{N −1}, (˜k_{N −1}), k_{N})

( ˜S)SME 6= 0
if and only if |S − k| ≤ S^{0} ≤ S + k

and M^{0}− M = q.

Both the Heisenberg-Dirac and biquadratic exchange are isotropic interactions. In fact, the corresponding Hamiltonians can be described by rank-0 tensor operators and thus have non zero matrix elements only with states with the same total spin quantum number S (∆S = 0 selection rule) and the same total spin projection M (∆M = 0 selection rule). The repesentative matrix can be decomposed into blocks depending only on the value of S and M . Differently, all anisotropic terms are described by rank- 2 tensor operators which have non zero matrix elements between state with different total spin S (∆S = 0,±1, ±2 selection rule). Therefore, their corresponding matrices can not be decomposed into blocks depending only on the value of the total spin S in account of the S-mixing between spin states with different values of S [38]. The single ion anisotropy can be written in terms of rank-2 single site ITO’s. Nevertheless, if the rhombic term of crystal field anisotropy can be neglected, then the representative ma- trix of CF interaction results to be composed of blocks depending only on the value of the total spin projection M . This reflects the selection rules ∆S = 0,±1, ±2, ∆M = 0.

Finally, the antisymmetric exchange term is the sum of ITO’s of rank k = 1, and its matrix elements are non zero only if ∆S = 0,±1.

The dimension of the matrices to be diagonalized for these systems increases dramat- ically by increasing the number of spin centers. In the next two sections two possible methods to solve this problem are described. Both methods take advantage from the